#------------------------------------------------------------------------------
#$Date: 2020-09-04 01:26:38 +0300 (Fri, 04 Sep 2020) $
#$Revision: 255835 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/36/4003666.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003666
loop_
_publ_author_name
'Shi, Shuangshuang'
'Lin, Chensheng'
'Yang, Guangsai'
'Cao, Liling'
'Li, Bingxuan'
'Yan, Tao'
'Luo, Min'
'Ye, Ning'
_publ_section_title
;
 A2Bi2(SeO3)3F2 (A = K and Rb): Excellent Mid-Infrared Nonlinear Optical
 Materials with Both Strong SHG Responses and Large Band Gaps
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.0c02837
_journal_year                    2020
_chemical_formula_sum            'Bi2 F2 K2 O9 Se3'
_chemical_formula_weight         915.04
_space_group_IT_number           8
_space_group_name_Hall           'C -2y'
_space_group_name_H-M_alt        'C 1 m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 93.076(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   12.8396(5)
_cell_length_b                   5.8831(3)
_cell_length_c                   7.6506(3)
_cell_measurement_reflns_used    1786
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      60.5760
_cell_measurement_theta_min      5.0380
_cell_volume                     577.07(4)
_computing_cell_refinement       'CrysAlisPro 1.171.40.59a (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.59a (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.59a (Rigaku OD, 2019)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0000
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'ROD, Synergy Custom system, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0312
_diffrn_reflns_av_sigmaI/netI    0.0374
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            1557
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.67
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_exptl_absorpt_coefficient_mu    40.697
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.13333
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.59a (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            Colourless
_exptl_crystal_density_diffrn    5.266
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Brick
_exptl_crystal_F_000             792
_refine_diff_density_max         3.956
_refine_diff_density_min         -7.234
_refine_diff_density_rms         1.128
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.04(2)
_refine_ls_extinction_coef       0.032(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_matrix_type           full
_refine_ls_number_parameters     85
_refine_ls_number_reflns         845
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0450
_refine_ls_R_factor_gt           0.0449
_refine_ls_shift/su_max          0.059
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1039P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1132
_refine_ls_wR_factor_ref         0.1134
_reflns_number_gt                843
_reflns_number_total             845
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm0c02837_si_002.cif
_cod_data_source_block           a
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Monoclinic' was changed to
'monoclinic' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_sg_symbol_H-M      'Cm   '
_cod_database_code               4003666
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x, -y, z'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.54595(6) 0.0000 0.52234(10) 0.0086(5) Uani 1 2 d S . .
Bi2 Bi 0.94969(8) 0.0000 -0.13469(11) 0.0089(4) Uani 1 2 d S . .
Se3 Se 0.8486(3) -0.5000 0.1468(5) 0.0129(8) Uani 1 2 d S . .
K1 K 0.2406(7) 0.0000 0.6996(14) 0.0140(16) Uani 1 2 d S . .
K2 K 0.6599(7) 0.0000 0.0403(11) 0.0153(18) Uani 1 2 d S . .
Se1 Se 0.5525(2) -0.5000 0.2950(5) 0.0106(7) Uani 1 2 d S . .
Se2 Se 0.8169(3) 0.0000 -0.5189(5) 0.0114(8) Uani 1 2 d S . .
F1 F 1.0684(11) -0.245(3) -0.2209(18) 0.019(3) Uani 1 1 d . . .
O1 O 0.8473(13) -0.273(3) 0.008(2) 0.025(4) Uani 1 1 d . . .
O2 O 0.6272(14) -0.288(3) 0.377(2) 0.015(3) Uiso 1 1 d . . .
O3 O 0.8904(14) 0.218(3) -0.438(2) 0.019(3) Uiso 1 1 d . . .
O4 O 0.7233(18) 0.0000 -0.377(3) 0.014(4) Uani 1 2 d S . .
O5 O 0.9749(19) -0.5000 0.225(3) 0.017(5) Uiso 1 2 d S . .
O6 O 0.5810(16) -0.5000 0.079(3) 0.010(5) Uani 1 2 d SU . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Bi1 O2 94.6(8) . 2 ?
O2 Bi1 O4 72.8(5) . 1_556 ?
O2 Bi1 O4 72.8(5) 2 1_556 ?
O2 Bi1 O5 72.6(6) . 3_455 ?
O2 Bi1 O5 72.6(6) 2 3_455 ?
O4 Bi1 O5 128.2(7) 1_556 3_455 ?
O2 Bi1 F1 142.3(5) . 3_456 ?
O2 Bi1 F1 84.4(5) 2 3_456 ?
O4 Bi1 F1 70.9(5) 1_556 3_456 ?
O5 Bi1 F1 140.6(4) 3_455 3_456 ?
O2 Bi1 F1 84.4(5) . 4_446 ?
O2 Bi1 F1 142.3(5) 2 4_446 ?
O4 Bi1 F1 70.9(5) 1_556 4_446 ?
O5 Bi1 F1 140.6(4) 3_455 4_446 ?
F1 Bi1 F1 74.5(7) 3_456 4_446 ?
O2 Bi1 O3 87.6(5) . 3_446 ?
O2 Bi1 O3 152.3(6) 2 3_446 ?
O4 Bi1 O3 133.5(4) 1_556 3_446 ?
O5 Bi1 O3 81.7(6) 3_455 3_446 ?
F1 Bi1 O3 110.4(5) 3_456 3_446 ?
F1 Bi1 O3 65.4(5) 4_446 3_446 ?
O2 Bi1 O3 152.3(6) . 4_456 ?
O2 Bi1 O3 87.6(5) 2 4_456 ?
O4 Bi1 O3 133.5(4) 1_556 4_456 ?
O5 Bi1 O3 81.7(6) 3_455 4_456 ?
F1 Bi1 O3 65.4(5) 3_456 4_456 ?
F1 Bi1 O3 110.4(5) 4_446 4_456 ?
O3 Bi1 O3 78.3(7) 3_446 4_456 ?
O2 Bi1 K2 50.5(4) . . ?
O2 Bi1 K2 50.5(4) 2 . ?
O4 Bi1 K2 84.7(6) 1_556 . ?
O5 Bi1 K2 43.5(6) 3_455 . ?
F1 Bi1 K2 133.8(3) 3_456 . ?
F1 Bi1 K2 133.8(3) 4_446 . ?
O3 Bi1 K2 114.8(4) 3_446 . ?
O3 Bi1 K2 114.8(4) 4_456 . ?
O2 Bi1 K1 114.1(5) . 3 ?
O2 Bi1 K1 48.8(5) 2 3 ?
O4 Bi1 K1 47.48(14) 1_556 3 ?
O5 Bi1 K1 120.9(3) 3_455 3 ?
F1 Bi1 K1 41.5(4) 3_456 3 ?
F1 Bi1 K1 97.5(4) 4_446 3 ?
O3 Bi1 K1 151.7(4) 3_446 3 ?
O3 Bi1 K1 87.9(4) 4_456 3 ?
K2 Bi1 K1 93.36(18) . 3 ?
O2 Bi1 K1 48.8(5) . 3_545 ?
O2 Bi1 K1 114.1(4) 2 3_545 ?
O4 Bi1 K1 47.48(14) 1_556 3_545 ?
O5 Bi1 K1 120.9(3) 3_455 3_545 ?
F1 Bi1 K1 97.5(4) 3_456 3_545 ?
F1 Bi1 K1 41.5(4) 4_446 3_545 ?
O3 Bi1 K1 87.9(4) 3_446 3_545 ?
O3 Bi1 K1 151.7(4) 4_456 3_545 ?
K2 Bi1 K1 93.36(18) . 3_545 ?
K1 Bi1 K1 93.3(2) 3 3_545 ?
O2 Bi1 K2 108.4(5) . 1_556 ?
O2 Bi1 K2 108.4(5) 2 1_556 ?
O4 Bi1 K2 53.5(6) 1_556 1_556 ?
O5 Bi1 K2 178.3(5) 3_455 1_556 ?
F1 Bi1 K2 38.9(3) 3_456 1_556 ?
F1 Bi1 K2 38.9(3) 4_446 1_556 ?
O3 Bi1 K2 97.0(4) 3_446 1_556 ?
O3 Bi1 K2 97.0(4) 4_456 1_556 ?
K2 Bi1 K2 138.2(2) . 1_556 ?
K1 Bi1 K2 60.02(14) 3 1_556 ?
K1 Bi1 K2 60.02(14) 3_545 1_556 ?
F1 Bi2 F1 80.9(8) . 2 ?
F1 Bi2 O6 73.8(5) . 3 ?
F1 Bi2 O6 73.8(5) 2 3 ?
F1 Bi2 O1 168.3(5) . 2 ?
F1 Bi2 O1 95.8(6) 2 2 ?
O6 Bi2 O1 94.4(5) 3 2 ?
F1 Bi2 O1 95.8(6) . . ?
F1 Bi2 O1 168.3(5) 2 . ?
O6 Bi2 O1 94.4(5) 3 . ?
O1 Bi2 O1 85.1(9) 2 . ?
F1 Bi2 O3 66.8(5) . 2 ?
F1 Bi2 O3 102.6(5) 2 2 ?
O6 Bi2 O3 140.5(5) 3 2 ?
O1 Bi2 O3 124.9(6) 2 2 ?
O1 Bi2 O3 86.3(5) . 2 ?
F1 Bi2 O3 102.6(5) . . ?
F1 Bi2 O3 66.8(5) 2 . ?
O6 Bi2 O3 140.5(5) 3 . ?
O1 Bi2 O3 86.3(5) 2 . ?
O1 Bi2 O3 124.9(6) . . ?
O3 Bi2 O3 56.2(7) 2 . ?
F1 Bi2 K1 40.7(4) . 1_654 ?
F1 Bi2 K1 40.7(4) 2 1_654 ?
O6 Bi2 K1 64.1(5) 3 1_654 ?
O1 Bi2 K1 133.8(4) 2 1_654 ?
O1 Bi2 K1 133.8(4) . 1_654 ?
O3 Bi2 K1 87.3(4) 2 1_654 ?
O3 Bi2 K1 87.3(4) . 1_654 ?
F1 Bi2 K2 139.4(4) . . ?
F1 Bi2 K2 139.4(4) 2 . ?
O6 Bi2 K2 114.9(5) 3 . ?
O1 Bi2 K2 45.8(4) 2 . ?
O1 Bi2 K2 45.8(4) . . ?
O3 Bi2 K2 93.6(4) 2 . ?
O3 Bi2 K2 93.6(4) . . ?
K1 Bi2 K2 179.0(2) 1_654 . ?
F1 Bi2 K1 83.8(4) . 3_544 ?
F1 Bi2 K1 144.5(4) 2 3_544 ?
O6 Bi2 K1 131.39(19) 3 3_544 ?
O1 Bi2 K1 104.8(4) 2 3_544 ?
O1 Bi2 K1 45.0(4) . 3_544 ?
O3 Bi2 K1 42.0(4) 2 3_544 ?
O3 Bi2 K1 85.8(4) . 3_544 ?
K1 Bi2 K1 120.24(18) 1_654 3_544 ?
K2 Bi2 K1 60.33(14) . 3_544 ?
F1 Bi2 K1 144.5(4) . 3_554 ?
F1 Bi2 K1 83.8(4) 2 3_554 ?
O6 Bi2 K1 131.39(19) 3 3_554 ?
O1 Bi2 K1 45.0(4) 2 3_554 ?
O1 Bi2 K1 104.8(4) . 3_554 ?
O3 Bi2 K1 85.8(4) 2 3_554 ?
O3 Bi2 K1 42.0(4) . 3_554 ?
K1 Bi2 K1 120.24(18) 1_654 3_554 ?
K2 Bi2 K1 60.33(14) . 3_554 ?
K1 Bi2 K1 90.7(2) 3_544 3_554 ?
F1 Bi2 K2 96.4(4) . 3 ?
F1 Bi2 K2 36.3(4) 2 3 ?
O6 Bi2 K2 47.89(17) 3 3 ?
O1 Bi2 K2 74.9(4) 2 3 ?
O1 Bi2 K2 134.1(4) . 3 ?
O3 Bi2 K2 138.9(4) 2 3 ?
O3 Bi2 K2 95.0(4) . 3 ?
K1 Bi2 K2 60.19(12) 1_654 3 ?
K2 Bi2 K2 119.23(14) . 3 ?
K1 Bi2 K2 179.1(2) 3_544 3 ?
K1 Bi2 K2 89.71(9) 3_554 3 ?
O5 Se3 O1 101.4(7) . 2_545 ?
O5 Se3 O1 101.4(7) . . ?
O1 Se3 O1 102.8(12) 2_545 . ?
O5 Se3 K1 130.1(8) . 3_544 ?
O1 Se3 K1 54.5(6) 2_545 3_544 ?
O1 Se3 K1 54.5(6) . 3_544 ?
O5 Se3 K2 130.50(10) . 1_545 ?
O1 Se3 K2 44.7(6) 2_545 1_545 ?
O1 Se3 K2 118.5(6) . 1_545 ?
K1 Se3 K2 66.26(14) 3_544 1_545 ?
O5 Se3 K2 130.50(10) . . ?
O1 Se3 K2 118.5(6) 2_545 . ?
O1 Se3 K2 44.7(6) . . ?
K1 Se3 K2 66.26(14) 3_544 . ?
K2 Se3 K2 98.9(2) 1_545 . ?
F1 K1 F1 63.7(7) 1_456 2_456 ?
F1 K1 O3 168.4(6) 1_456 4_456 ?
F1 K1 O3 110.6(5) 2_456 4_456 ?
F1 K1 O3 110.6(5) 1_456 3_446 ?
F1 K1 O3 168.4(6) 2_456 3_446 ?
O3 K1 O3 72.9(7) 4_456 3_446 ?
F1 K1 O1 113.8(5) 1_456 3_456 ?
F1 K1 O1 86.0(5) 2_456 3_456 ?
O3 K1 O1 74.7(5) 4_456 3_456 ?
O3 K1 O1 105.6(6) 3_446 3_456 ?
F1 K1 O1 86.0(5) 1_456 4_446 ?
F1 K1 O1 113.8(5) 2_456 4_446 ?
O3 K1 O1 105.6(6) 4_456 4_446 ?
O3 K1 O1 74.7(5) 3_446 4_446 ?
O1 K1 O1 53.2(7) 3_456 4_446 ?
F1 K1 O4 58.3(5) 1_456 3_446 ?
F1 K1 O4 120.5(6) 2_456 3_446 ?
O3 K1 O4 123.6(6) 4_456 3_446 ?
O3 K1 O4 52.4(6) 3_446 3_446 ?
O1 K1 O4 128.3(6) 3_456 3_446 ?
O1 K1 O4 75.1(5) 4_446 3_446 ?
F1 K1 O4 120.5(6) 1_456 3_456 ?
F1 K1 O4 58.3(5) 2_456 3_456 ?
O3 K1 O4 52.4(6) 4_456 3_456 ?
O3 K1 O4 123.6(6) 3_446 3_456 ?
O1 K1 O4 75.1(5) 3_456 3_456 ?
O1 K1 O4 128.3(6) 4_446 3_456 ?
O4 K1 O4 156.3(9) 3_446 3_456 ?
F1 K1 O2 67.1(4) 1_456 4_445 ?
F1 K1 O2 92.2(5) 2_456 4_445 ?
O3 K1 O2 104.1(6) 4_456 4_445 ?
O3 K1 O2 76.2(5) 3_446 4_445 ?
O1 K1 O2 177.3(5) 3_456 4_445 ?
O1 K1 O2 129.4(4) 4_446 4_445 ?
O4 K1 O2 54.4(5) 3_446 4_445 ?
O4 K1 O2 102.3(6) 3_456 4_445 ?
F1 K1 O2 92.2(5) 1_456 3_455 ?
F1 K1 O2 67.1(4) 2_456 3_455 ?
O3 K1 O2 76.2(5) 4_456 3_455 ?
O3 K1 O2 104.1(6) 3_446 3_455 ?
O1 K1 O2 129.4(4) 3_456 3_455 ?
O1 K1 O2 177.3(5) 4_446 3_455 ?
O4 K1 O2 102.3(6) 3_446 3_455 ?
O4 K1 O2 54.4(5) 3_456 3_455 ?
O2 K1 O2 47.9(6) 4_445 3_455 ?
F1 K1 Se2 85.1(3) 1_456 3_446 ?
F1 K1 Se2 142.1(4) 2_456 3_446 ?
O3 K1 Se2 95.8(4) 4_456 3_446 ?
O3 K1 Se2 27.8(4) 3_446 3_446 ?
O1 K1 Se2 128.1(4) 3_456 3_446 ?
O1 K1 Se2 82.8(3) 4_446 3_446 ?
O4 K1 Se2 27.8(4) 3_446 3_446 ?
O4 K1 Se2 137.6(5) 3_456 3_446 ?
O2 K1 Se2 54.2(3) 4_445 3_446 ?
O2 K1 Se2 95.0(4) 3_455 3_446 ?
F1 K1 Se2 142.1(4) 1_456 3_456 ?
F1 K1 Se2 85.1(3) 2_456 3_456 ?
O3 K1 Se2 27.8(4) 4_456 3_456 ?
O3 K1 Se2 95.8(4) 3_446 3_456 ?
O1 K1 Se2 82.8(3) 3_456 3_456 ?
O1 K1 Se2 128.1(4) 4_446 3_456 ?
O4 K1 Se2 137.6(5) 3_446 3_456 ?
O4 K1 Se2 27.8(4) 3_456 3_456 ?
O2 K1 Se2 95.0(4) 4_445 3_456 ?
O2 K1 Se2 54.2(3) 3_455 3_456 ?
Se2 K1 Se2 112.0(3) 3_446 3_456 ?
F1 K2 F1 67.0(7) 4_445 3_455 ?
F1 K2 O5 91.5(6) 4_445 3_455 ?
F1 K2 O5 91.5(6) 3_455 3_455 ?
F1 K2 O1 124.6(5) 4_445 2 ?
F1 K2 O1 87.7(5) 3_455 2 ?
O5 K2 O1 139.6(4) 3_455 2 ?
F1 K2 O1 87.7(5) 4_445 . ?
F1 K2 O1 124.6(5) 3_455 . ?
O5 K2 O1 139.6(4) 3_455 . ?
O1 K2 O1 66.9(6) 2 . ?
F1 K2 O2 146.4(6) 4_445 2 ?
F1 K2 O2 103.6(5) 3_455 2 ?
O5 K2 O2 55.6(5) 3_455 2 ?
O1 K2 O2 85.4(4) 2 2 ?
O1 K2 O2 121.1(6) . 2 ?
F1 K2 O2 103.6(5) 4_445 . ?
F1 K2 O2 146.4(6) 3_455 . ?
O5 K2 O2 55.6(5) 3_455 . ?
O1 K2 O2 121.1(6) 2 . ?
O1 K2 O2 85.4(4) . . ?
O2 K2 O2 65.7(6) 2 . ?
F1 K2 O6 54.7(5) 4_445 . ?
F1 K2 O6 117.4(6) 3_455 . ?
O5 K2 O6 70.6(4) 3_455 . ?
O1 K2 O6 143.0(5) 2 . ?
O1 K2 O6 76.3(5) . . ?
O2 K2 O6 111.9(5) 2 . ?
O2 K2 O6 49.7(5) . . ?
F1 K2 O6 117.4(6) 4_445 1_565 ?
F1 K2 O6 54.7(5) 3_455 1_565 ?
O5 K2 O6 70.6(4) 3_455 1_565 ?
O1 K2 O6 76.3(5) 2 1_565 ?
O1 K2 O6 143.0(5) . 1_565 ?
O2 K2 O6 49.7(5) 2 1_565 ?
O2 K2 O6 111.9(5) . 1_565 ?
O6 K2 O6 140.0(8) . 1_565 ?
F1 K2 O4 54.1(5) 4_445 . ?
F1 K2 O4 54.1(5) 3_455 . ?
O5 K2 O4 137.2(7) 3_455 . ?
O1 K2 O4 70.9(5) 2 . ?
O1 K2 O4 70.9(5) . . ?
O2 K2 O4 146.8(3) 2 . ?
O2 K2 O4 146.8(3) . . ?
O6 K2 O4 100.8(4) . . ?
O6 K2 O4 100.8(4) 1_565 . ?
F1 K2 Se1 130.2(4) 4_445 1_565 ?
F1 K2 Se1 78.3(3) 3_455 1_565 ?
O5 K2 Se1 53.85(19) 3_455 1_565 ?
O1 K2 Se1 86.6(3) 2 1_565 ?
O1 K2 Se1 142.1(4) . 1_565 ?
O2 K2 Se1 25.4(3) 2 1_565 ?
O2 K2 Se1 86.0(4) . 1_565 ?
O6 K2 Se1 123.1(4) . 1_565 ?
O6 K2 Se1 26.1(4) 1_565 1_565 ?
O4 K2 Se1 126.90(18) . 1_565 ?
F1 K2 Se1 78.3(3) 4_445 . ?
F1 K2 Se1 130.2(4) 3_455 . ?
O5 K2 Se1 53.85(19) 3_455 . ?
O1 K2 Se1 142.1(4) 2 . ?
O1 K2 Se1 86.6(3) . . ?
O2 K2 Se1 86.0(4) 2 . ?
O2 K2 Se1 25.4(3) . . ?
O6 K2 Se1 26.1(4) . . ?
O6 K2 Se1 123.1(4) 1_565 . ?
O4 K2 Se1 126.90(18) . . ?
Se1 K2 Se1 100.5(2) 1_565 . ?
O2 Se1 O2 96.2(12) . 2_545 ?
O2 Se1 O6 102.2(8) . . ?
O2 Se1 O6 102.2(8) 2_545 . ?
O2 Se1 K2 53.3(6) . . ?
O2 Se1 K2 123.2(6) 2_545 . ?
O6 Se1 K2 53.6(3) . . ?
O2 Se1 K2 123.2(6) . 1_545 ?
O2 Se1 K2 53.3(6) 2_545 1_545 ?
O6 Se1 K2 53.6(3) . 1_545 ?
K2 Se1 K2 100.5(2) . 1_545 ?
O2 Se1 K1 51.2(6) . 3_545 ?
O2 Se1 K1 51.2(6) 2_545 3_545 ?
O6 Se1 K1 128.5(7) . 3_545 ?
K2 Se1 K1 100.56(17) . 3_545 ?
K2 Se1 K1 100.56(17) 1_545 3_545 ?
O4 Se2 O3 99.8(8) . . ?
O4 Se2 O3 99.8(8) . 2 ?
O3 Se2 O3 98.9(11) . 2 ?
O4 Se2 K1 57.6(2) . 3_554 ?
O3 Se2 K1 50.3(6) . 3_554 ?
O3 Se2 K1 128.4(6) 2 3_554 ?
O4 Se2 K1 57.6(2) . 3_544 ?
O3 Se2 K1 128.4(6) . 3_544 ?
O3 Se2 K1 50.3(6) 2 3_544 ?
K1 Se2 K1 112.0(3) 3_554 3_544 ?
O4 Se2 K2 102.1(8) . 1_554 ?
O3 Se2 K2 125.3(6) . 1_554 ?
O3 Se2 K2 125.3(6) 2 1_554 ?
K1 Se2 K2 105.6(2) 3_554 1_554 ?
K1 Se2 K2 105.6(2) 3_544 1_554 ?
Bi2 F1 Bi1 125.1(6) . 3_544 ?
Bi2 F1 K2 114.6(6) . 3_545 ?
Bi1 F1 K2 106.1(6) 3_544 3_545 ?
Bi2 F1 K1 107.3(6) . 1_654 ?
Bi1 F1 K1 101.8(5) 3_544 1_654 ?
K2 F1 K1 97.6(5) 3_545 1_654 ?
Se3 O1 Bi2 145.8(9) . . ?
Se3 O1 K2 111.0(7) . . ?
Bi2 O1 K2 98.4(6) . . ?
Se3 O1 K1 97.6(7) . 3_544 ?
Bi2 O1 K1 100.5(6) . 3_544 ?
K2 O1 K1 88.2(5) . 3_544 ?
Se1 O2 Bi1 117.5(9) . . ?
Se1 O2 K1 103.7(7) . 3_545 ?
Bi1 O2 K1 96.7(5) . 3_545 ?
Se1 O2 K2 101.3(7) . . ?
Bi1 O2 K2 94.7(6) . . ?
K1 O2 K2 143.6(6) 3_545 . ?
Se2 O3 Bi1 148.3(9) . 3_554 ?
Se2 O3 Bi2 94.5(7) . . ?
Bi1 O3 Bi2 102.4(6) 3_554 . ?
Se2 O3 K1 101.9(8) . 3_554 ?
Bi1 O3 K1 102.3(5) 3_554 3_554 ?
Bi2 O3 K1 97.1(6) . 3_554 ?
Se2 O4 Bi1 120.3(12) . 1_554 ?
Se2 O4 K1 94.5(5) . 3_554 ?
Bi1 O4 K1 97.1(5) 1_554 3_554 ?
Se2 O4 K1 94.5(5) . 3_544 ?
Bi1 O4 K1 97.1(5) 1_554 3_544 ?
K1 O4 K1 156.3(9) 3_554 3_544 ?
Se2 O4 K2 147.9(12) . . ?
Bi1 O4 K2 91.8(7) 1_554 . ?
K1 O4 K2 80.4(4) 3_554 . ?
K1 O4 K2 80.4(4) 3_544 . ?
Se3 O5 Bi1 129.9(12) . 3_545 ?
Se3 O5 K2 129.3(12) . 3_545 ?
Bi1 O5 K2 100.8(9) 3_545 3_545 ?
Se1 O6 Bi2 120.2(11) . 3_445 ?
Se1 O6 K2 100.3(5) . . ?
Bi2 O6 K2 99.3(5) 3_445 . ?
Se1 O6 K2 100.3(5) . 1_545 ?
Bi2 O6 K2 99.3(5) 3_445 1_545 ?
K2 O6 K2 140.0(8) . 1_545 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O2 2.310(16) . ?
Bi1 O2 2.310(16) 2 ?
Bi1 O4 2.36(2) 1_556 ?
Bi1 O5 2.40(3) 3_455 ?
Bi1 F1 2.475(14) 3_456 ?
Bi1 F1 2.475(14) 4_446 ?
Bi1 O3 2.626(17) 3_446 ?
Bi1 O3 2.626(17) 4_456 ?
Bi1 K2 4.040(8) . ?
Bi1 K1 4.046(7) 3 ?
Bi1 K1 4.046(7) 3_545 ?
Bi1 K2 4.150(8) 1_556 ?
Bi2 F1 2.225(15) . ?
Bi2 F1 2.225(15) 2 ?
Bi2 O6 2.29(2) 3 ?
Bi2 O1 2.378(15) 2 ?
Bi2 O1 2.378(15) . ?
Bi2 O3 2.727(17) 2 ?
Bi2 O3 2.727(17) . ?
Bi2 K1 4.008(10) 1_654 ?
Bi2 K2 4.022(8) . ?
Bi2 K1 4.136(7) 3_544 ?
Bi2 K1 4.136(7) 3_554 ?
Bi2 K2 4.164(6) 3 ?
Se3 O5 1.70(3) . ?
Se3 O1 1.706(16) 2_545 ?
Se3 O1 1.706(16) . ?
Se3 K1 3.622(11) 3_544 ?
Se3 K2 3.870(6) 1_545 ?
Se3 K2 3.870(6) . ?
K1 F1 2.736(17) 1_456 ?
K1 F1 2.736(17) 2_456 ?
K1 O3 2.789(18) 4_456 ?
K1 O3 2.789(18) 3_446 ?
K1 O1 2.98(2) 3_456 ?
K1 O1 2.977(19) 4_446 ?
K1 O4 3.005(5) 3_446 ?
K1 O4 3.005(5) 3_456 ?
K1 O2 3.06(2) 4_445 ?
K1 O2 3.06(2) 3_455 ?
K1 Se2 3.547(6) 3_446 ?
K1 Se2 3.547(6) 3_456 ?
K2 F1 2.714(16) 4_445 ?
K2 F1 2.714(16) 3_455 ?
K2 O5 2.83(2) 3_455 ?
K2 O1 2.916(19) 2 ?
K2 O1 2.916(19) . ?
K2 O2 3.129(18) 2 ?
K2 O2 3.129(18) . ?
K2 O6 3.130(8) . ?
K2 O6 3.130(8) 1_565 ?
K2 O4 3.34(2) . ?
K2 Se1 3.826(6) 1_565 ?
K2 Se1 3.826(5) . ?
Se1 O2 1.671(16) . ?
Se1 O2 1.671(16) 2_545 ?
Se1 O6 1.71(2) . ?
Se1 K2 3.826(6) 1_545 ?
Se1 K1 3.823(10) 3_545 ?
Se2 O4 1.66(2) . ?
Se2 O3 1.690(17) . ?
Se2 O3 1.690(17) 2 ?
Se2 K1 3.547(6) 3_554 ?
Se2 K1 3.547(6) 3_544 ?
Se2 K2 3.835(9) 1_554 ?
F1 Bi1 2.475(14) 3_544 ?
F1 K2 2.714(16) 3_545 ?
F1 K1 2.736(17) 1_654 ?
O1 K1 2.977(19) 3_544 ?
O2 K1 3.06(2) 3_545 ?
O3 Bi1 2.626(17) 3_554 ?
O3 K1 2.789(18) 3_554 ?
O4 Bi1 2.36(2) 1_554 ?
O4 K1 3.005(5) 3_554 ?
O4 K1 3.005(5) 3_544 ?
O5 Bi1 2.40(3) 3_545 ?
O5 K2 2.83(2) 3_545 ?
O6 Bi2 2.29(2) 3_445 ?
O6 K2 3.130(8) 1_545 ?
